Heterobimetallic Coordination Polymers Based on the [Pt(SCN)4]2- and [Pt(SeCN)4]2- Building Blocks
Masayuki Kobayashi; Didier Savard; Andrew R. Geisheimer; Ken Sakai; Daniel B. Leznoff; Inorganic Chemistry 52 (2013) 4842–4852; doi:10.1021/ic302360b

data_4334581
_publ_contact_author_address
; 
Leznoff, Daniel B.
Department of Chemistry
Simon Fraser University
Burnaby, British Columbia
Canada         V5A 1S6
;
_publ_contact_author_email       dleznoff@sfu.ca
_publ_contact_author_fax         +1-778-782-3765
_publ_contact_author_name        'Daniel B. Leznoff'
_publ_contact_author_phone       +1-778-782-4887
_publ_section_title
;
 Heterobimetallic Coordination Polymers Based on the [Pt(SCN)4]2- and
 [Pt(SeCN)4]2- Building Blocks
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              4842
_journal_page_last               4852
_journal_paper_doi               10.1021/ic302360b
_journal_volume                  52
_journal_year                    2013
_chemical_formula_moiety         'C22.67 H14.67 Mn0.67 N6.67 Pt0.67 S2.67'
_chemical_formula_sum            'C22.67 H14.67 Mn0.67 N6.67 Pt0.67 S2.67'
_chemical_formula_weight         632.60
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_atom_sites_solution_hydrogens   difmap
_atom_sites_solution_primary     direct
_cell_angle_alpha                90
_cell_angle_beta                 112.315(5)
_cell_angle_gamma                90
_cell_formula_units_Z            6
_cell_length_a                   19.387(4)
_cell_length_b                   8.4368(19)
_cell_length_c                   23.520(5)
_cell_measurement_reflns_used    0
_cell_measurement_temperature    293
_cell_measurement_theta_max      0
_cell_measurement_theta_min      0
_cell_volume                     3558.9(13)
_computing_cell_refinement       'Bruker Apex2'
_computing_data_collection       'Bruker Apex2'
_computing_data_reduction        'USER DEFINED DATA REDUCTION'
_computing_molecular_graphics    'CAMERON (Watkin et al., 1996)'
_computing_publication_material  'CRYSTALS (Betteridge et al., 2003)'
_computing_structure_refinement  'CRYSTALS (Betteridge et al., 2003)'
_computing_structure_solution    'SIR92 (Altomare et al., 1994)'
_diffrn_ambient_temperature      293
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.997
_diffrn_measurement_device       Serial
_diffrn_measurement_device_type  Unknown
_diffrn_measurement_method       \w/2\q
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.043
_diffrn_reflns_limit_h_max       22
_diffrn_reflns_limit_h_min       -22
_diffrn_reflns_limit_k_max       9
_diffrn_reflns_limit_k_min       -9
_diffrn_reflns_limit_l_max       27
_diffrn_reflns_limit_l_min       -26
_diffrn_reflns_number            56806
_diffrn_reflns_theta_full        24.359
_diffrn_reflns_theta_max         24.359
_diffrn_reflns_theta_min         1.135
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    4.558
_exptl_absorpt_correction_T_max  1.0000
_exptl_absorpt_correction_T_min  1.0000
_exptl_absorpt_correction_type   empirical
_exptl_crystal_colour            orange
_exptl_crystal_density_diffrn    1.771
_exptl_crystal_description       plate
_exptl_crystal_F_000             1852
_exptl_crystal_size_max          0.48
_exptl_crystal_size_mid          0.27
_exptl_crystal_size_min          0.05
_refine_diff_density_max         1.00
_refine_diff_density_min         -0.45
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.2109
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     455
_refine_ls_number_reflns         3249
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0736
_refine_ls_R_factor_gt           0.0357
_refine_ls_shift/su_max          0.0004811
_refine_ls_shift/su_mean         0.0000274
_refine_ls_structure_factor_coef F
_refine_ls_weighting_details
;
 Method= Modified Sheldrick 
 w=1/[\s^2^(F) + ( 0.03P)^2^ + 0.00P] 
 ,where P=(max(Fo,0) + 2Fc)/3 
;
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_all         0.0929
_refine_ls_wR_factor_gt          0.0498
_refine_ls_wR_factor_ref         0.0474
_reflns_limit_h_max              20
_reflns_limit_h_min              -22
_reflns_limit_k_max              9
_reflns_limit_k_min              0
_reflns_limit_l_max              27
_reflns_limit_l_min              0
_reflns_number_gt                3465
_reflns_number_total             5808
_reflns_threshold_expression     I>2.0\s(I)
_oxford_diffrn_Wilson_B_factor   4.66
_oxford_diffrn_Wilson_scale      418.25
_oxford_refine_ls_r_factor_ref   0.0333
_oxford_refine_ls_scale          0.05983(12)
_oxford_reflns_number_all        5808
_oxford_reflns_threshold_expression_ref I>2.5\s(I)
_cod_data_source_file            ic302360b_si_002_10.cif
_cod_data_source_block           C34H22N10MnPtS4
_cod_original_cell_volume        3558.8(14)
_cod_original_sg_symbol_H-M      'P 1 21/c 1 '
_cod_database_code               4334581